General

Property | Temperature | Value |
---|---|---|

Density | 20.0 °C | 10.5 g/cm³ Show Material materials with Density of 10.5 g/cm³ |

Mechanical

Property | Temperature | Value | Comment |
---|---|---|---|

Elastic modulus | -195.0 °C | 89 GPa Show Material materials with Elastic modulus of 89 GPa | |

20.0 °C | 80 GPa Show Material materials with Elastic modulus of 80 GPa | ||

200.0 °C | 77 GPa Show Material materials with Elastic modulus of 77 GPa | ||

400.0 °C | 67 GPa Show Material materials with Elastic modulus of 67 GPa | ||

600.0 °C | 57 GPa Show Material materials with Elastic modulus of 57 GPa | ||

800.0 °C | 46 GPa Show Material materials with Elastic modulus of 46 GPa | ||

900.0 °C | 40 GPa Show Material materials with Elastic modulus of 40 GPa | ||

Hardness, Vickers | 20.0 °C | 70 [-] Show Material materials with Hardness, Vickers of 70 [-] | |

Poisson's ratio | 23.0 °C | 0.37 [-] Show Material materials with Poisson's ratio of 0.37 [-] | Typical for Silver |

Shear modulus | 20.0 °C | 26 GPa Show Material materials with Shear modulus of 26 GPa |

Thermal

Property | Temperature | Value | Comment |
---|---|---|---|

Coefficient of thermal expansion | 100.0 °C | 1.79E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.79E-5 1/K | |

150.0 °C | 1.86E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.86E-5 1/K | ||

200.0 °C | 1.91E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.91E-5 1/K | ||

250.0 °C | 1.92E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.92E-5 1/K | ||

300.0 °C | 1.94E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.94E-5 1/K | ||

350.0 °C | 1.97E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.97E-5 1/K | ||

400.0 °C | 1.99E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.99E-5 1/K | ||

450.0 °C | 2.01E-5 1/K Show Material materials with Coefficient of thermal expansion of 2.01E-5 1/K | ||

500.0 °C | 2.04E-5 1/K Show Material materials with Coefficient of thermal expansion of 2.04E-5 1/K | ||

600.0 °C | 2.12E-5 1/K Show Material materials with Coefficient of thermal expansion of 2.12E-5 1/K | ||

700.0 °C | 2.25E-5 1/K Show Material materials with Coefficient of thermal expansion of 2.25E-5 1/K | ||

800.0 °C | 2.36E-5 1/K Show Material materials with Coefficient of thermal expansion of 2.36E-5 1/K | ||

900.0 °C | 2.43E-5 1/K Show Material materials with Coefficient of thermal expansion of 2.43E-5 1/K | ||

Unlock all property charts | |||

Melting point | 962 °C Show Material materials with Melting point of 962 °C | Typical for Silver | |

Specific heat capacity | 23.0 °C | 234 - 251 J/(kg·K) Show Material materials with Specific heat capacity of 234 - 251 J/(kg·K) | Typical for Silver |

Thermal conductivity | -233.0 °C | 1050 W/(m·K) Show Material materials with Thermal conductivity of 1050 W/(m·K) | |

-173.0 °C | 475 W/(m·K) Show Material materials with Thermal conductivity of 475 W/(m·K) | ||

-73.0 °C | 441 W/(m·K) Show Material materials with Thermal conductivity of 441 W/(m·K) | ||

20.0 °C | 419 W/(m·K) Show Material materials with Thermal conductivity of 419 W/(m·K) | ||

127.0 °C | 426 W/(m·K) Show Material materials with Thermal conductivity of 426 W/(m·K) | ||

327.0 °C | 411 W/(m·K) Show Material materials with Thermal conductivity of 411 W/(m·K) | ||

527.0 °C | 397 W/(m·K) Show Material materials with Thermal conductivity of 397 W/(m·K) | ||

927.0 °C | 383 W/(m·K) Show Material materials with Thermal conductivity of 383 W/(m·K) | ||

Unlock all property charts |

Electrical

Property | Temperature | Value |
---|---|---|

Electrical conductivity | 20.0 °C | 6.00E+7 S/m Show Material materials with Electrical conductivity of 6.00E+7 S/m |

Electrical resistivity | 20.0 °C | 1.67E-8 - 1.8E-8 Ω·m Show Material materials with Electrical resistivity of 1.67E-8 - 1.8E-8 Ω·m |

Chemical properties

Property | Value |
---|---|

Silver | 99.97 % Show Material materials with Silver of 99.97 % |